Group 2 metal bis(arenecarbochalcogenoate)(crown ether) complexes: isolation and structural analysis.
Tatematsu, Yoshiharu; Kato, Shinzi; Nakata, Norio; Ebihara, Masahiro; Niyomura, Osamu; Sugamata, Koh; Yukimoto, Mariko; Minoura, Mao; Dalton transactions (Cambridge, England : 2003) 47 (2018) 9787–9794; doi:10.1039/c8dt01959b

data_7046876
_publ_section_title
;
 Group 2 metal bis(arenecarbochalcogenoate)(crown ether) complexes:
 isolation and structural analysis.
;
_journal_issue                   29
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              9787
_journal_page_last               9794
_journal_paper_doi               10.1039/c8dt01959b
_journal_volume                  47
_journal_year                    2018
_chemical_formula_moiety         'C28 H38 O8 Se2 Sr'
_chemical_formula_sum            'C28 H38 O8 Se2 Sr'
_chemical_formula_weight         748.12
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2yn'
_space_group_name_H-M_alt        'P 1 21/n 1'
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2018-06-21 deposited with the CCDC.
2018-06-26 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 99.17(2)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.686(2)
_cell_length_b                   13.944(2)
_cell_length_c                   14.556(2)
_cell_measurement_reflns_used    25
_cell_measurement_temperature    193(2)
_cell_measurement_theta_max      12.3
_cell_measurement_theta_min      10.5
_cell_volume                     1540.1(5)
_computing_cell_refinement       'MSC/AFC Diffractometer Control'
_computing_data_collection       'MSC/AFC Diffractometer Control'
_computing_data_reduction        'teXsan: PROCESS (MSC)'
_computing_molecular_graphics    'Mercury (Macrae et al., 2008)'
_computing_publication_material
'Yadokari-XG 2009 (Wakita, Nemoto et al., 2009)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SIR97 (Altomare et al., 1999)'
_diffrn_ambient_temperature      193(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Rigaku AFC7R'
_diffrn_measurement_method       \w-2\q
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.7107
_diffrn_reflns_av_R_equivalents  0.0380
_diffrn_reflns_av_unetI/netI     0.1511
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            4646
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        25.241
_diffrn_reflns_theta_max         27.496
_diffrn_reflns_theta_min         2.035
_diffrn_standards_decay_%        1.40
_diffrn_standards_interval_count 150
_diffrn_standards_number         3
_exptl_absorpt_coefficient_mu    4.159
_exptl_absorpt_correction_T_max  0.999
_exptl_absorpt_correction_T_min  0.916
_exptl_absorpt_correction_type   psi-scan
_exptl_absorpt_process_details   '(North, Phillips & Mathews, 1968)'
_exptl_crystal_colour            'pale yellow'
_exptl_crystal_density_diffrn    1.613
_exptl_crystal_description       prismatic
_exptl_crystal_F_000             752
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.17
_exptl_crystal_size_min          0.17
_refine_diff_density_max         0.533
_refine_diff_density_min         -0.860
_refine_diff_density_rms         0.122
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.997
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     179
_refine_ls_number_reflns         3516
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.997
_refine_ls_R_factor_all          0.1559
_refine_ls_R_factor_gt           0.0465
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0335P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0813
_refine_ls_wR_factor_ref         0.1060
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1757
_reflns_number_total             3516
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c8dt01959b2.cif
_cod_data_source_block           14b
_cod_depositor_comments
'Adding full bibliography for 7046874--7046878.cif.'
_cod_database_code               7046876
_shelx_shelxl_version_number     2014/7
_shelx_estimated_absorpt_t_min   0.490
_shelx_estimated_absorpt_t_max   0.538
_shelx_res_checksum              60783